In this letter, the production of multi-phase WO3 and WO3- x (where x could vary between 0.1 and 0.3) nanostructures synthesized by CO2-laser pyrolysis technique at varying laser wavelengths (9.22-10.82 mm) and power densities (17-110 W/cm2) is reported. The average spherical particle sizes for the wavelength variation samples ranged between 113 and 560 nm, and the average spherical particle sizes for power density variation samples ranged between 108 and 205 nm. Synthesis of W18O49 (= WO2.72) stars by this method is reported for the first time at a power density and wavelength of 2.2 kW/cm2 and 10.6 μm, respectively. It was found that more concentrated starting precursors result in the growth of hierarchical structures such as stars, whereas dilute starting precursors result in the growth of simpler structures such as wires.
Tungsten trioxide is known as a 'smart material', because it exhibits excellent electrochromic, photochromic and gasochromic properties. Nano-sized tungsten trioxide has been applied in many nano-photonic devices for applications such as photo-electro-chromic windows , sensor devices [2, 3] and optical modulation devices . Many techniques for synthesizing nano-sized tungsten trioxide have been reported [5–8] and this article concerns with laser pyrolysis.
Laser pyrolysis is more advantageous than most methods because the experimental orientation does not allow the reactants to make contact with any side-walls, so that the products are of high quality and purity . Laser pyrolysis is based on photon-induced chemical reactions, which is believed to rely on a resonant interaction between a laser beam's emission line and a precursor's absorption band, such that a photochemical reaction is activated . The photochemical reaction enables an otherwise inaccessible reaction pathway towards a specific product, either by dissociation, ionization or isomerisation of the precursor compound. It was shown [8, 11] that low laser power densities can also achieve the same desired products as the high power densities, presumably because of the way photon-energy is distributed into the energy levels of the precursor.
In this letter, the formation of W18O49 (= WO2.72) and the effect of the laser power, the wavelength on the morphology and structural properties of tungsten oxide nano-structured and thin films are reported.
The laser pyrolysis experimental setup was discussed in detail in , and a schematic description of the experiment during laser-precursor interaction is depicted in Figure 1. The laser pyrolysis method is carried out within a custom-made stainless steel chamber at atmospheric pressure. A wavelength tunable Continuous Wave CO2 laser was used in the experiments (Edinburgh Instruments, model PL6, 2 Bain Square, Kirkton Campus, Livingston, UK) and the beam was focused into the reaction chamber with a 1-m radius of curvature concave mirror which is effectively a lens with a focal length of 500 mm. For low power densities, an unfocused beam was used by replacing the concave mirror with a flat mirror. An IR-detector (Ophir-Spiricon, model PY-III-C-A, Ophir Distribution Center, Science-Based Industrial Park, Har Hotzvim, Jerusalem, Israel) was used to trace out the laser beam profile at various propagation distances from the flat or concave mirror to determine the beam properties.
The laser power was varied using a polarization-based attenuator, and the wavelength variation was achieved with an intra-cavity mounted grating in the laser. The different wavelengths were identified using a spectrum analyzer (Macken Instruments Inc., model 16A, Coffey Lane, Santa Rosa, California, USA) and the power output was measured with a power meter (Coherent Inc., 5100 Patrick Henry Drive, Santa Clara, CA 95054, USA).
The synthesis of WO3 and WO3- x commenced by mixing 0.1 g of greyish-blue anhydrous tungsten hexachloride (WCl6, >99.9%, Sigma Aldrich, 3050 Spruce Street, St. Louis, MO 63103, USA) powder in 100 mL of absolute ethanol (C2H5OH, >99.9%, Sigma Aldrich) to give a tungsten ethoxide W(OC2H5)6 starting precursor . Optical absorption properties of the precursor were determined using a Perkin Elmer Spotlight 400 FTIR Imaging System in the wavelength range 500-4000 cm-1.
The liquid precursor was decanted into an aerosol generator (Micro Mist, model EN, Research Triangle Park, NC 27709, USA) which was attached to the laser pyrolysis system via a multiflow nozzle that allows argon gas to carry the stream of very fine precursor droplets (5 μm droplet diameter according to the manufacturer) into the laser beam. Acetylene (C2H2) sensitizer gas and argon encasing gas flowed adjacent to the precursor, guiding it towards a substrate. The gas flow rates are chosen such that the ablated precursor collects on the substrate after interacting with the laser.
The sample was annealed for 17 h at 500°C under argon atmosphere . Morphology studies were carried out using a Jeol JSM-5600 Scanning Electron Microscopy (SEM) microscope (using the secondary electron mode). Raman spectroscopy was carried out using a Jobin-Yvon T64000 Raman Spectrograph with a wavelength of 514.5 nm from an argon ion laser set at a laser power of 0.384 mW at the sample to minimize local heating of the sample during the Raman analysis. X-ray diffraction (XRD) was carried out using a Philips Xpert powder diffractometer equipped with a CuKα wavelength of 154.184 pm. The reproducibility of the experimental procedure was not verified.
When the CO2 laser beam was focused with a 1-m radius of curvature mirror, it produced a minimum beam radius or a beam waist of 1.2 mm, and at a laser power of 50 W on the 10.6-μm emission line, a power density of 2.2 kW/cm2 was achieved. These parameters were consistent with those obtained when synthesizing WO3 nanowires using a very dilute precursor of 27 μM . Laser pyrolysis of the more concentrated 2.5 mM precursor showed many uniform agglomerations composed of nanospheres (40 nm) before annealing, as depicted in the SEM micrograph in the inset of Figure 2. The sample was annealed, and from the agglomerates, stars grew with six points as seen in the SEM micrographs of Figure 2.
The Raman and XRD spectra of the samples containing the stars are shown in Figure 3. The stars were not visible under the Raman microscope and so various spots were analyzed on the sample. The Raman study shows that the sample is amorphous after annealing, and the lack of a dominant peak at 800 cm-1 suggests the absence of monoclinic phase tungsten trioxide and possibly oxygen deficiency [13, 14]. The Raman peaks found near 224 cm-1, 288 cm-1 and 320 cm-1 are indicative of a W-O-W stretching mode of a tungsten oxide. The Raman peak at 700 cm-1 is designated to the bridging O-W-O vibrations in tungsten trioxide, and the asymmetry in this phonon peak shows that there are a number of phonons confined in the tungsten oxide layer of particles. This indicates that the product is composed of particles less than 20 nm in size [15, 16]. The peak near 960 cm-1 is assigned to the W6+ = O symmetric stretching mode.
The XRD studies revealed peaks at 23° and 24° diffraction angles which suggests a tungsten oxide compound, but the lack of a triplet peak confirms the absence of monoclinic tungsten trioxide . The broad hump at 22° resulted from SiO2 of the substrate, and this substantially decreased the signal-to-noise ratio making it difficult to identify the peaks. XRD peaks at 11, 40 and 64° diffraction angles are also evident in tungsten oxides , but the 44° diffraction angle suggests that the tungsten oxide has a deficiency of oxygen . Based on the information from Raman spectroscopy and XRD, the most probable stoichiometry of this sample is monoclinic phase W18O49 (= WO2.72). According to the Powder Diffraction File (PDF 00-005-0392) that best matches the XRD spectrum in Figure 3, the lattice constants a, b and c are 18.28, 3.78 and 13.98 Å, respectively and the lattice angles are α = γ = 90° and β = 115.20°. The Miller indices are shown on the XRD spectrum in Figure 3.
Previously solid-vapour-solid (SVS)  and solution-liquid-solid (SLS)  mechanisms were proposed to explain the growth of nanowires of tungsten trioxide and platinum, respectively. Since the tungsten trioxide nanowires were grown with a low precursor concentration using a similar laser beam and laser parameters, the precursor concentration is seemingly the main contributor to hierarchical structure. This was confirmed by the 100 times more concentrated precursor that was used for the growth of the stars. The six-sided stars that were grown in Figure 2 looked very similar to lead (II) sulphide (PbS) stars that were grown by a concentration difference and gradient (CDG) technique . This CDG technique used a high local concentration of one reactant mixed with a low concentration of another reactant under ambient conditions, where the high concentration favoured the thermodynamic conditions for crystal growth and the low concentration resulted in a diffusion-controlled kinetic environment for growth of hierarchical structures.
It is possible that due to a Gaussian laser beam profile, which has a high intensity at the beam's centre and low intensity at the edges, the region of intensity in the beam experienced by the precursor could vary the concentration of the decomposed material. It is speculated that this variation in concentration could have led to the growth of the hierarchical structures according to the CDG technique. The growth of stars has also been reported before for gold and molybdenum oxide [21, 22], but not as yet for tungsten oxide. The literature proposes that star-shaped structures can be grown from agglomerates of more simple nanoforms under an inert atmosphere, which conditions were similar for this experiment [21, 22]. One growth mechanism of nanostructures could be due to Gibbs-Thompson effect [9, 23, 24], which proposes that the size of the critical radius is dependent on the precursor concentration and explains the increase (Ostwald ripening) or decrease (Tiller's formula) in size of nanostructures.
The higher concentration probably provided a critical radius which resulted in simple nanoforms and the growth of stars as opposed to a lower concentration which resulted in microspheres and the growth of wires. It is speculated that the critical radius influences the thermodynamic and kinetic conditions as predicted by the CDG technique. Thus, the laser beam properties together with the relative precursor concentration contribute to the growth of stars. Some stars may form with four-sides and others with six-sides depending on the crystalline plane arrangement and the elements composing the structures . It is not yet understood if the observed deficiency of oxygen plays a role in the formation of the six-sided stars or if the higher tungsten content, with a predominant valency of +6, has some correlation with the number of sides formed.
It is thought that acetylene gas acts as a photosensitizer  in laser pyrolysis, yet no evidence of absorption in the laser wavelength range 9.19-10.82 μm was found. This was verified by passing the acetylene gas through the laser beam at atmospheric pressure, and monitoring the power change during this interaction. The laser power did not appear to show any change, which implied that no radiation was absorbed by this gas. This does not, however, discount the possibility of some short-lived metastable state in acetylene induced by the laser which was undetectable by the power meter. The argon-precursor mixture, however, showed a change in power which indicated that the radiation was being absorbed, and the maximum absorbance was found at a wavelength of 9.54 μm. The absorbance of the precursor was given by the ratio of the laser power before laser-precursor interaction to the power observed during laser-precursor interaction.
Figure 4 shows the absorbance by the precursor as a function of wavelength with the corresponding part of the FTIR transmission spectrum of tungsten ethoxide. This determination gives us an idea if the laser pyrolysis mechanism is a resonant process or if the precursor is decomposed by collisions with excited photosensitizer molecules. However, the results indicate that the laser energy gets transferred to the precursor and should cause decomposition by a resonant process, thus leading to the formation of the predicted products. Therefore, acetylene probably provides a reducing atmosphere in the laser-precursor interaction that influences the reaction pathway towards the formation of the products.
To determine how the laser wavelength plays a role in laser pyrolysis, it was varied between 9.19 and 10.84 μm at a constant power of 30 W and power density of 51.2 W/cm2. The lower power density was achieved by replacing the focusing mirror with a flat mirror to obtain a beam radius of 6.11 mm. The low power density was chosen such that all the R- and P-branches of the CO2 laser supplied a constant power output for the varying wavelengths. It was also assumed that at such low power density, minimum heating effects are involved in the laser-precursor interaction. It was found that only the 10.48-μm wavelength formed monoclinic phase WO3 according to the Raman and XRD spectra shown in Figure 5 with the corresponding SEM micrograph.
The nanosphere diameters of this sample, which were easiest to measure on SEM micrograph, were distributed in the range 50-250 nm as depicted in inset of Figure 5, and micron-sized fibres were also present in this sample. The theory speculates that if the laser wavelength is resonant with the C-O absorption band of the precursor (W-O-C2H5), then the C-O bond would break and lead to the formation of tungsten oxide. However, FTIR showed that the C-O absorption band is found between 9.00-9.38 μm (see Figure 4), and despite argon carrier gas presumably broadening the precursor absorption bands to some extent , the result could correspond to a non-resonant energy transfer. A 10.48-μm wavelength photon carries 0.1 eV of energy, and so 29 photons are required to dissociate a C-O bond  which corresponds to a multi-photon process. It is known, however, that tungsten ethoxide precursor can form WO3 upon heat treatment , which implies that the 10.48-μm wavelength could have had similar effects as annealing had. We believe that the shorter wavelengths, which had higher energy photons, dissociated various bonds which led to the formation of triclinic phase or a mixture of monoclinic and triclinic phase WO3- x where x can vary between 0.1 and 0.3, depending on the laser parameters. It was also observed that the morphology of the samples became more randomized and of a disordered arrangement as the wavelength increased, and this is believed to be an effect of a corresponding decrease in energy.
Unlike the increasing wavelength, the increase in power density led to more ordered and shaped nanostructures, presumably because of the increase in energy rate. The 10.6 μm wavelength appeared to favour the formation of monoclinic phase tungsten oxide Furthermore, it was observed that at high enough power densities, it was more likely for helping nanostructure growth. At such low power densities (17-110 W/cm2) on the 10.6 μm wavelength, the particle sizes did not show a decrease with increasing power density as predicted  for the higher power density range (1-100 kW/cm2). The nanosphere diameters of this sample were found to be in the range 150-400 nm as depicted in inset of Figure 6. It was observed that the overall particle sizes were smaller for the power variation experiment, while the wavelength variation experiment showed larger particle sizes. The increase in power density did not always favour the formation of WO3, and since the photon energy was constant, only the number of photons per unit time varied.
Figure 6 shows the Raman and XRD spectra with the corresponding SEM micrograph of a sample prepared at a power density of 85 W/cm2 at the 10.6-μm wavelength, which appeared to form a monoclinic phase WO3 according to the characteristic peaks.
Table 1 summarizes all the results obtained for the varying laser parameters. The average particle sizes observed for the wavelength variation was in the range 113-560 nm, while the average particle sizes for the power density variation were in the range 108-205 nm. The compositions of some samples were uncertain, and so it is written as WO3- x where x most likely attains values between 0.1 and 0.3. There were no obvious trends as to how the laser parameters affected the product size or composition, and thus, it is believed that some possible competing reactions taking place during the laser-precursor interaction or during annealing.
Six-sided monoclinic phase WO2.72 stars were synthesized by laser pyrolysis technique using a more concentrated starting precursor and near-Gaussian laser beam profile. The higher concentrated precursors are required to obtain hierarchical structures as predicted by the literature. Laser wavelengths above 10 μm seem to favour the formation of stoichiometric WO3, but only at certain power densities, presumably to overcome possible competing reactions. Owing to the nature of photochemical reactions and the many stoichiometries and multi-phases that tungsten oxides can form, some product compositions were written as WO3- x where x most probably assumes values between 0.1 and 0.3. The higher power densities were found to be essential for the further growth of structures and for smaller particle sizes. The authors now have an idea of the possible shapes of nanostructures that can be synthesized with possible chemical compositions, and the determination of the electrical and optical properties of these structures to observe possible unique characteristics allows for the tailoring of sensor devices that operate at room temperature for example.
Conflict of interest
The authors declare that they have no conflict of interests.
Bittencourt C, Landers R, Llobet E, Molas G, Correig X, Silva MAP, Sueiris JE, Calderer J: Effects of Oxygen Partial Pressure and Annealing Temperature on the Formation of Sputtered Tungsten Oxide Films. Electrochem Soc 2002, 149: H81. 10.1149/1.1448821
Kawasaki H, Namba J, Iwatsuji K, Suda Y, Wada K, Ebihara K, Ohshima T: NO x gas sensing properties of tungsten oxide thin films synthesized by pulsed laser deposition method. Appl Surf Sci 2002, 197–198: 547–551. 10.1016/S0169-4332(02)00333-1
Guidi V, Butturi MA, Blo M, Carotta MC, Galliera S, Giberti A, Malagù C, Martinelli G, Piga M, Sacerdoti M, Vendemiati B: Aqueous and alcoholic syntheses of tungsten trioxide powders for NO 2 detection. Sens Actuators B 2004, 100: 277. 10.1016/j.snb.2003.12.055
Wang SW, Chou TC, Liu CC: Nano-crystalline tungsten oxide NO 2 sensor. Sens Actuators B 2003, 94: 343. 10.1016/S0925-4005(03)00383-6
Wang XP, Yang BQ, Zhang HX, Feng PX: Tungsten Oxide Nanorods Array and Nanobundle Prepared by Using Chemical Vapor Deposition Technique. Nanoscale Res Lett 2007, 2: 405–409. 10.1007/s11671-007-9075-3
Rajagopal S, Nataraj D, Mangalaraj D, Djaoued Y, Robichaud J, Khyzhun O: Controlled Growth of WO 3 Nanostructures with Three Different Morphologies and Their Structural, Optical, and Photodecomposition Studies. Nanoscale Res Lett 2009, 4: 1335–1342. 10.1007/s11671-009-9402-y
Mwakikunga BW, Forbes A, Sideras-Haddad E, Scriba M, Manikandan E: Self assembly and properties of C:WO 3 nano-platelets and C:VO 2 /V 2 O 5 triangular capsules of C:VO 2 /V 2 O 5 fullerenes and quantum dots produced by laser solution photolysis. Nanoscale Res Lett 2010, 5: 389–397. 10.1007/s11671-009-9494-4
Mwakikunga BW, Forbes A, Sideras-Haddad E, Arendse C: Optimization, yield studies and morphology of WO 3 nanowires synthesized by laser pyrolysis in C 2 H 2 and O 2 ambients - validation of a new growth mechanism. Nanoscale Res Lett 2008, 3: 372–380. 10.1007/s11671-008-9169-6
Haggerty JS, Cannon WR: Sinterable powders from laser-driven reactions. In Laser Induced Chemical Reactions. Edited by: J. I. Steinfield. New York, Plenum Press; 1981:165–241.
Mwakikunga BW, Forbes A, Sideras-Haddad E, Erasmus RM, Katumba G, Masina B: Synthesis of tungsten oxide nanostructures by laser pyrolysis. Int J Nanopart 2008, 1: 185–200. 10.1504/IJNP.2008.020895
Bowden CM, Stettler JD, Witriol NM: An excitation model for laser-induced photochemical reactions. J Phys B Atom Mol Phys 1977, 10: 1789. 10.1088/0022-3700/10/9/028
Sakka S: Handbook of Sol-Gel Science and Technology: Processing, Characterization and Applications. Boston: Kluwer Academic Publishers; 2004.
Lu DY, Chen J, Zhou J, Deng SZ, Xu NS, Xu JB: Raman spectroscopic study of oxidation and phase transition in W 18 O 49 nanowires. J Raman Spectrosc 2007, 38: 176–180. 10.1002/jrs.1620
Lu DY, Chen J, Deng SZ, Xu NS, Zhang WH: The most powerful tool for the structural analysis of tungsten suboxide nanowires: Raman spectroscopy. J Mater Res 2008, 23: 402–408. 10.1557/jmr.2008.0056
Mwakikunga BW, Sidera-Haddad E, Forbes A, Arndse C: Raman spectroscopy of WO 3 nano-wires and thermo-chromism study of VO 2 belts produced by ultrasonic spray and laser pyrolysis techniques. Phys Status Solidi A 2004, 205: 150–154.
Arora AK, Rajalakshmi M, Ravindran TR: Phonon Confinement in Nanostructured Materials. In Encyclopedia of Nanoscience and Nanotechnology, Volume X. Edited by: Nalwa HS. Los Angeles: American Scientific Publishers; 2003:1–13.
Ganesan R, Gedanken A: Synthesis of WO 3 nanoparticles using a biopolymer as a template for electrocatalytic hydrogen evolution. Nanotechnology 2008, 19: 025702. 10.1088/0957-4484/19/02/025702
Microelectronic capacitor with capacitor plate layer formed of tungsten rich tungsten oxide material2002. [http://www.surechem.org] Patent 6456482
Chen J, Wiley BJ, Xia Y: One-dimensional nanostructures of metals: large-scale synthesis and some potential applications. Langmuir 2007, 27: 4120–4129. 10.1021/la063193y
Chu H, Li X, Chen G, Jin Z, Zhang Y, Li Y: Inorganic hierarchical nanostructures induced by concentration difference and gradient. Nano Res 2008, 1: 213–220. 10.1007/s12274-008-8024-5
Kharissova OV, Kharisov BI, García TH, Méndez UO: A Review on Less-common Nanostructures. Synth React Inorg Met-Org Nano-Met Chem 2009, 39: 662–684.
Khademi A, Azimirad R, Zavarian AA, Moshfegh AZ: Growth and Field Emission Study of Molybdenum Oxide Nanostars. J Phys Chem C 2009, 44: 19298–19304. 10.1021/jp9056237
Qin-bo W, Finsy R, Hai-bo X, Xi L: On the critical radius in generalized Ostwald ripening. J Zhejiang Univ 2005, 6B: 705–707. 10.1631/jzus.2005.B0705
Tiller WA: The Science of Crystallization: Microscopic Interfacial Phenomenon. New York: Cambridge University Press; 1991.
El-Diasty F: Simulation of CO 2 laser pyrolysis during preparation of SiC nanopowders. Opt Commun 2004, 241: 121–135. 10.1016/j.optcom.2004.07.006
Glockler G: Carbon Halogen Bond Energies and Bond Distances. J Phys Chem 1958, 62: 1049–1054. 10.1021/j150567a006
Bomatí-Miguel O, Zhao XQ, Martelli S, Di Nunzio PE, Veintemillas-Verdaguer S: Modeling of the laser pyrolysis process by means of the aerosol theory: Case of iron nanoparticles. J Appl Phys 2010, 107: 014906.
MG carried out all the experiments in conjunction with LS. MG also initiated the first draft manuscript. BWM assisted with the production of thin films by laser pyrolysis, characterization, analysis, interpretation of experimental results and manuscript handling. AF performed the optical alignment of the laser pyrolysis and discussion of the manuscript. ESH contributed through discussion of the manuscript and RE provided the Raman spectral data from all samples.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
About this article
Cite this article
Govender, M., Shikwambana, L., Mwakikunga, B.W. et al. Formation of tungsten oxide nanostructures by laser pyrolysis: stars, fibres and spheres. Nanoscale Res Lett 6, 166 (2011). https://doi.org/10.1186/1556-276X-6-166